Magnetization and Magnetic Change of Length. 561 



Table IV. 



Nickel- Steels. 



70-32% 



>0-72°/o 



46% 



36% 



29-24% 



29% 



28-74 % 



28-32 % 



Ordinary Temperatur 



Liquid Air Temperature. 



H 

 B 

 W 



21 3-4 31-2 

 2675 7069 11370 

 886 3510 5353 



39 4-6 38- 

 4104 6790 13910 

 2015 4300 11160 



2-9 4- 



1350 3845 



202 1969 



7- 



7783 

 5836 



4-0 9-5 39-7 

 2782 6910 11520 

 1264 5290 9404 



H 07 6-9 780 

 B 749 2774 419 

 W 147 109 155 



H 



B 



Yv 



1-3 9-7 33 7 

 1099 2807 3654 

 106 395 393 



089 4-96 53-3 

 1261 3054 4662 

 58 189 322 



H 

 B 

 W 



46-5 218-6 

 373 1184 

 45 16 





H 



25-3 



62-3 



148-7 



26-64 % 



B 



64 



173 



354 





W 



51 



276 



703 





TT 



35-6 



85-0 



126 



2440% 



B 



94 



215 



295 





W 



153 



511 



731 



2404 % 



102-7 



30-3 



331 : 608 



1110 2586 



244-6 

 926 

 4108 



H 

 B 

 W 



2-5 

 2628 

 9841 



4-9 

 6850 

 4140 



302 

 11550 

 7494 







H 

 B 

 W 



2-6 

 919 

 1026 



4-9 

 3493 

 1970 



6-8 

 7677 

 6867 



H 

 B 



W 



5-8 

 2581 

 1654 



95 



6948 

 8000 



310 



12800 

 19303 



H 

 B 

 W 





5-0 

 507 

 79 



14-5 

 2132 

 2271 



22-6 



5188 

 13120 



i 



1 



H 

 B 

 W 





11-8 



1938 



1888 



19 3 

 39»>4 

 7439 



57-2 

 8394 

 28060 



H 



B 

 W 



145 

 1552 

 1.396 



232 

 3406 



7864 



60-2 



8076 

 36900 





| 



E 

 B 

 W 



\ 17-1 2£6 89- 

 1180 3212 8783 

 1309 10520' 63550 



Phil' Mag. S. 6. Vol. 10. No. 59. Nov. 1905. 



2Q 



